Abstract
A central prospect of antiferromagnetic spintronics is to exploit magnetic properties that are unavailable with ferromagnets. However, this poses the challenge of accessing such properties for readout and control. To this end, lightinduced manipulation of the transient ground state, e.g. by changing the magnetic anisotropy potential, opens promising pathways towards ultrafast deterministic control of antiferromagnetism. Here, we use this approach to trigger a coherent rotation of the entire longrange antiferromagnetic spin arrangement about a crystalline axis in GdRh_{2}Si_{2} and demonstrate deterministic control of this rotation. Our observations can be explained by a laserinduced shift of the direction of the Gd spins’ local magnetic anisotropy, and allow for a quantitative description of the transient magnetic anisotropy potential.
Introduction
Antiferromagnets have attracted great interest in recent years due to their potential to push forward the field of spintronics^{1}. A central advantage of antiferromagnetic (AF) over ferromagnetic (FM) spintronics arises from their selfcancelling spin arrangement with zero net moment, rendering them largely insensitive to external fields. Such stability holds great potential for devices (e.g. for digital storage density and longevity), but also poses significant challenges to implement magnetic functionality, requiring new approaches to interact with magnetic order. To this end, a key promise of AF spintronics is to exploit and control magnetic properties that are unique to antiferromagnets, such as the ordering wave vector or changes to the spin arrangement itself^{2,3,4}. Another potential benefit of AF spintronics stems from their enhanced magnetic resonance frequencies, promising efficient control of the magnetic state by ultrashort pulses. While in thermal equilibrium a number of approaches for control of AF spintronic systems have been demonstrated^{2}, more recently also significant progress has been made in manipulating magnetism in AF and ferrimagnetic systems using ultrashort THz^{5,6,7,8} or visible^{9,10} light pulses. However, many of these approaches relied on very specific sample geometries or material properties, for example, noncentrosymmetric lattice symmetries^{2,11}.
Another possible route for control of antiferromagnetism using optical stimulation is to utilize the local anisotropy of the AF ordered ions to steer the magnetic state of a system. For example, different configurations that are sufficiently close in energy may be susceptible to thermally driven effects on the local (singleion) magnetic anisotropy. A sudden rise in heat induced by a femtosecond laser excitation can abruptly change this anisotropy, to which the longrange AF order would then respond by realigning according to a new easy axis. In this work, we demonstrate deterministic control of this effect in the prototypical Atype antiferromagnet GdRh_{2}Si_{2}. The system is an exemplary case of a magnetically soft XY antiferromagnet^{12}, due to the low anisotropy of the closed Gd 4f shell, which has no orbital angular momentum (L = 0). Its weak magnetic anisotropy makes it ideal for our study, as it allows efficient modification of the anisotropy potential of the Gd ions through ultrafast photoexcitation. Following the excitation, we observe a coherent and deterministic rotation of the entire AF arrangement of Gd spins about a crystalline axis, without loss of the longrange coherence of the AF order. Further analysis of the coherent rotations of the AF structure also allows us to fully determine the local magnetic anisotropy potential.
Results
Equilibrium AF behaviour
Before investigating the response to laser excitation, we begin by characterizing the equilibrium behaviour of the AF order in GdRh_{2}Si_{2}. We study its magnetic structure, which consists of FM Gd layers (ab planes) stacked antiparallel to each other along the [001] direction^{13} (the tetragonal axis, Fig. 1a), using resonant Xray diffraction (RXD)^{14,15}. Tuning the incoming Xrays to the Gd M_{5} edge (3d_{5/2} → 4f transitions, see Supplementary Fig. 1), we gain sensitivity exclusively to the longrange AF order of the Gd 4f spins by studying the (001) magnetic reflection, which is forbidden for diffraction from the crystal lattice. Since we diffract from ordered spins, the scatterers are not isotropic and the orientation of the spin arrangement relative to the light polarization vector can cause the intensity to depend on the azimuthal angle Ψ (Fig. 1a). Detecting the scattered intensity as function of Ψ therefore allows us to completely determine the orientation of the Gd 4f spin moments m, which are aligned along an easy axis within the ab plane, at an angle φ relative to the [100] direction (Fig. 1b). The normalized diffraction intensity of the (001) reflection at various temperatures is shown in Fig. 1c. It exhibits a remarkable shift of the cosineshaped function with temperature, indicating a change of the magnetic easy axis. Our data can be well described by a magnetic structure factor that depends on m and φ as^{16,17}:
Here, m and φ are functions of either temperature (T) or pumpprobe delay time (t, see following). Using Eq. (1) we extract the temperaturedependent behaviour of m(T) and φ(T) from the data in Fig. 1c and find that m(T) fits well to a meanfield behaviour for S = 7/2 (see “Methods”), and that φ(T) changes significantly in the range 30–70 K (Fig. 1d). This corresponds to a gradual rotation of the aforementioned easy axis in the direction from ~[110] towards [010] upon heating (see Fig. 1b). We emphasize that this is a collective rotation of the entire AF spin structure about the [001] axis (i.e. the material remains AF with vanishing net moment).
To understand this effect, we consider the possible contributions to magnetic anisotropy in GdRh_{2}Si_{2}. Because the Gd 4f shell is spherical (L = 0), its anisotropy terms are typically very weak, and only two contributions can occur: from onsite exchange coupling to the conduction electrons, which do experience magnetic anisotropy (and mediate the Ruderman–Kittel–Kasuya–Yosida (RKKY) interaction), and from dipolar interactions^{18,19}. The dipolar contribution is not expected to contribute to the rotation effect (it itself depends on the spins’ orientation), leaving the conduction electrons. Therefore, to gain insight on the observed rotation, the electron density at the Fermi level was calculated for several temperatures. The effect of temperature was simulated as a spin disorder using the disordered local moment (DLM) approximation (see “Methods”). Figure 2a presents the realspace distribution of the electron density within a Gd plane, in which the Gd 5d orbital character is dominant. Four different levels of spin disorder are shown, representing different temperatures. For low spin disorder (low temperature) strong hybridization between the Gd 5d states and the Si sp bands causes the 5d orbitals to extend along the [110] direction (Si ions are the closest to Gd ions). Upon increasing spin disorder (heating), the extent of the 5d orbitals along [110] shrinks, causing a reduction in hybridization along [110] in favour of [010] (indicated by dotted lines in Fig. 2a). This change in 5d anisotropy is imprinted via the strong exchange coupling to the 4f states, directly influencing their anisotropy by shifting the overall easyaxis angle φ in the direction from [110] to [010] (and symmetry equivalents). This explanation for the observed change in the magnetic anisotropy is also corroborated by the calculated easyaxis angle shown for several spin disorders in Fig. 2b. It qualitatively reproduces the experimental trend of Fig. 1d, demonstrating the validity of our approach (note that φ in Fig. 2b is plotted against spin disorder, in contrast to temperature in Fig. 1d). The rotation effect is also reflected in variations of the Fermi surface in reciprocal space, where degenerate and nearly degenerate states contribute most strongly to the magnetic anisotropy energy^{20}. Upon heating, the direction of highest degeneracy shifts from [110] towards [010] due to an energy shift in the bands near the X point (see Supplementary Note 2).
AF behaviour upon ultrafast excitation
Having established the equilibrium behaviour of the magnetic structure, we now optically excite the system in order to test if we can induce a similar behaviour on ultrafast time scales, as sketched in Fig. 3a. We studied the temporal evolution of the AF structure at a base temperature of 11 K, where m ≈ m_{0} and φ ≈ 58°. We excited the system with 1.55 eV laser pulses, which arrive at delay times t before the femtosecond Xray probe pulse. The (001) intensity I(t, Ψ) is found to either increase or decrease depending on Ψ, but no change is observed in the shape or position of the diffraction peak (Fig. 3b, c). This allows us to track the evolution of I(t, Ψ) by measuring the timedependent intensity at the maximum of the diffraction peak only. The evolution of I(t, Ψ) with time is strongly fluence dependent, exhibiting both an oscillatory feature and a suppression in magnitude (Fig. 3d).
Similar to the equilibrium case, the temporal evolution of φ(t) and m(t) can be disentangled using Eq. (1) by measuring I(t, Ψ) for several values of Ψ. We measured pumpprobe delay scans at four values of Ψ, as indicated in Fig. 3a, and used these results to fit Eq. (1) for each value of t (see Supplementary Note 3). We found that Eq. (1) provides a good description of the transient behaviours of φ(t) and m(t) (Fig. 4a, b). m(t) exhibits suppression and recovery dynamics, reminiscent of the ultrafast demagnetization dynamics found in various magnetic systems^{21}, while φ(t) exhibits a combination of a continuous rotation and a superimposed coherent oscillation, corresponding to a collective rotation of the entire AF structure upon photoexcitation (Fig. 3a). We note here that 90° magnetic domains can occur in this tetragonal system and can be identified by their intensity’s Ψ dependence and their transient response. Corrections to intensity from overlapping domains have been applied to some datasets (see “Methods” and Supplementary Note 4). The influence of possible deviations from Eq. (1) is discussed in Supplementary Note 3, in which the most general form of the transient magnetic response is given.
We now discuss the dynamics of m and φ in more detail. A hierarchy of the quantities discussed in the next sections is shown in Fig. 5a for guidance.
The demagnetization of m(t) (Fig. 4a) is well described by two exponential decay channels (see “Methods”), “fast” and “slow”, with corresponding time constants τ and demagnetization amplitudes d. The fast channel occurs on a subpicosecond time scale (300–600 fs, see example in the inset of Fig. 4a), while the slow channel is ~100 times slower (20–40 ps) and accounts for most of the demagnetization amplitude (d_{slow} > d_{fast}, Fig. 5c). Similar biexponential demagnetization has been reported for Lanthanide metals, both for AF^{22,23} and FM^{22,24,25} cases. In all cases, the highspeed subpicosecond channel accounts for a small fraction of total demagnetization, while the slower channel (i.e. a few ps to tens of ps) accounts for the rest. The appearance of two time scales has been interpreted as one demagnetization process that is initially fast due to the presence of hot electrons, which have not yet thermalized with the lattice, and then becomes slower once the electrons and phonons have thermalized^{26,27}. The time scales we observe (Fig. 5b) are in very good agreement with those found for both demagnetization channels of FM Gd metal^{24,28} and other Gdbased materials^{9,25}. Demagnetization amplitudes d exhibit a linear behaviour up to a critical fluence F_{C} (Fig. 5c). In this linear range, the time scales τ slow down, a feature associated with the rise in susceptibility near the ordering temperature^{29}. For the slow channel, this occurs at F/F_{C} ≈ 1.
We now discuss the transient rotation dynamics of the AF structure, observed through φ(t) (Fig. 4b). The main feature is a gradual reorientation of the AF structure towards higher φ values, analogous to the rotation upon heating (dashed lines in Fig. 4b). An additional coherent oscillation of the AF structure is observed superimposed on the gradual rotation. We stress that these behaviours are collective and coherent motions of the entire AF spin structure, and in analogy to the behaviour upon heating, represent a variation in the ions’ local magnetic anisotropy. The total change in φ can be described as
Here, Φ and Ω represent the reorientation and the oscillation, respectively (indicated in Fig. 4b). Unlike in the demagnetization data, no subpicosecond dynamics are observed. The gradual reorientation Φ(t) occurs on time scales τ_{φ} of tens of ps (Fig. 5d), similar to the values of τ_{slow}. At late delays the reorientation begins to recover on a slower time scale τ_{rec}, such that the whole process can be described as
The amplitude Φ_{0} and time constant τ_{φ} both grow with fluence. Such a dependence is a direct example of a controllable variation in an AF spin arrangement. To demonstrate deterministic control, the inset of Fig. 4b presents the fluence dependence of φ(t) − φ(0) at a delay of 1 ns (this delay was chosen such that all oscillations are clearly damped). A linear fluence dependence is observed in a wide fluence range, reaching complete rotation of the AF structure towards the [010] direction (Δφ > 30°) for the highest fluences.
Further insight into the underlying timedependent magnetic anisotropy potential can be gained from the coherent oscillations Ω(t). This term exhibits fluencedependent frequencies ω of 6–12 of GHz (Fig. 5d), and is damped on time scales τ_{damp} well below the recovery of Φ(t). It is well described in the form
Solid lines in Fig. 4b represent best fits to Eqs. (2)–(4). The observed rotations are reminiscent of displacive excitations of coherent phonons (DECPs)^{30}, in which a steplike change in a vibrational potential triggers coherent phonon oscillations (see “Methods”). In analogy, we describe the local inplane magnetic anisotropy of the Gd spins as a potential U(φ) of magnitude K, centred around the equilibrium angle φ_{0} as
In this picture, the coherent spin oscillations are triggered by the rapid change of the easyaxis direction φ_{0} expressed through Φ(t) in Eq. (3), as depicted in the cartoon in Fig. 5e. Equation 4 represents a solution of the equation of motion within this transient anisotropy potential, describing an oscillation of the AF structure around the transient easy axis, at a frequency ω corresponding to the transient value of the magnetic anisotropy constant K. The extracted values of K (see “Methods”) are presented in Fig. 5f as a function of Φ_{0}, the amplitude of the transient easyaxis rotation (Eq. (3)). They are remarkably close to those of Gd metal^{18}, and the corresponding anisotropy fields reach 0.24 T, in good agreement with results by Sichelschmidt et al.^{31}.
Discussion
Our method provides a complete description of the transient magnetic anisotropy, which exhibits a linear relation \(K \propto {{\noexpand\iPhi}}_0\) in Fig. 5f, demonstrating that both quantities (easyaxis angle and anisotropy strength) change together upon excitation. Assuming the transient system to be in a thermally equilibrated state, our transient values of K can be interpreted as a measure of the equilibrium anisotropy potential. This assumption is reasonable, considering that the reorientation occurs over tens of ps, which is substantially longer than typical eph thermalization time scales in metals of only a few ps^{32}. Thus, our results demonstrate not only a method to control the AF spin structure using light, but also to probe the anisotropy potential of an antiferromagnet through a displacive excitation, which can be understood as an AF Γpoint magnon^{33}.
In this work, we have demonstrated the optical manipulation of the local (singleion) magnetic anisotropy via its temperature dependence. Beyond such thermal effects, strong variations in this energy landscape could also be achieved by other means, such as directly tuning magnetic interactions, varying the crystal field, distorting the local environment with an excited phonon mode and more. Such approaches could also offer faster response times to the excitation. Ultimately, the purpose is to embed such functionalities in spintronic devices. For example, in the context of magnetic memory such effects could facilitate ultrafast alloptical control of the pinning direction in writehead spin valves, or enable ultrafast steering of spin current directions in exchangebiased layers. Understanding controllable magnetic properties is challenging with antiferromagnets because of their inaccessibility through conventional means. The insight gained on U(φ) through our approach was enabled by the relatively slow GHz frequencies characteristic of our model material system. Antiferromagnets that are candidates for applications typically exhibit THz frequencies^{34}, which renders similar effects more appealing for future devices, but also more challenging to identify. The effects we present may also be applicable beyond the scope of antiferromagnets, because of the Gd ions’ combination of high spin moment and low anisotropy. For example, the easy axis of Gd metal is also known to rotate upon warming by up to 60°^{35}, suggesting that optically induced reorientation towards a transient easy axis could also occur. This and other similarities between our observations and other Gdbased magnets suggest that optical control of AF order may be possible for other Gd systems. Since Gd is commonly employed in applications requiring its high 4f moment, this property may prove as useful for the design of deterministically controllable spintronic devices.
Methods
Sample preparation
Samples were cleaved single crystals of GdRh_{2}Si_{2}, grown as described in ref. ^{13}. Due to the layered crystal structure, the cleaved sample face normal is precisely parallel to the tetragonal [001] axis. The crystals used were ~1 mm^{3} in size, with faces much larger than the beam sizes.
Resonant Xray diffraction
All experiments were conducted by fulfilling the Bragg condition for the (001) magnetic reflection using incoming photon energies near the Gd M_{5} absorption edge (~1190 eV). All experiments were conducted with σpolarized incoming light. Correspondingly, Eq. (1) considers only the σ → π′ channel (σ → σ′ is 0 by symmetry for magnetic E1–E1 events). From the shape of the (001) reflection around the M_{5} edge, we estimate an effective Xray probe depth of 26 nm (see Supplementary Note 1). The angle Ψ is 0° when the [100] direction is in the scattering plane.
Equilibrium RXD experiments
Experiments were conducted at beamline X11MA of the Swiss Light Source^{36}, using the RESOXS end station^{37} and at beamline ID32 at the ESRF^{38}.
Following Aharoni^{39}, in Fig. 1d the temperature dependence of m(T) was fit to a meanfield approximation of the form
The tabulated parameters for S = 7/2 are a = −1.478 × 10^{−3} and b = 2.7221 × 10^{−2}. The temperature dependence of φ(T) was fit to an error function of the form:
Timeresolved RXD experiments
Experiments were conducted in a UHV scattering chamber using ultrashort Xray pulses from the femtoslicing facility at beamline UE56/1ZPM^{40} at the HelmholzZentrum Berlin. The zone plate monochromator used in this experiment provided an energy resolution of 4 eV (see Supplementary Note 1).
The pumpprobe experimental scheme was conducted at 3 kHz using 1.55 eV (800 nm) ppolarized pump pulses. The Xray repetition rate is 6 kHz such that between every pumped event an unpumped signal is recorded, and no average heating was observed. The detector is an avalanche photodiode (APD). The 1190 and 1.55 eV pulses arrive nearly collinearly, but the APD does not collect the pump photons, which are blocked by an Al foil. The 1.55 and 1190 eV spot profiles were set to (166 ± 26 × 321 ± 60) and (170 ± 66 × 170) μm^{2 }^{41}, respectively.
The detection scheme allowed for singlephoton counting, such that collected intensities represent photon counts per second. As such, the error bars in Fig. 3b–d are taken as \({\mathrm{{\Delta}}}I = \sqrt I\). Reciprocal space scans such as those in Fig. 3b, c were collected for every fluence at several delays, and no broadening or shifting of the peaks was observed. Therefore, only the peak heights were collected in time traces.
The timeresolved experiments were conducted at four azimuths at 45° intervals: Ψ = 15°, 60°, 105° and 150°. The probed areas on the surface were chosen to ensure a singledomain state: twodimensional scans of the sample surface were taken before and after excitation. Chosen areas were large and homogeneous, and exhibited a uniform response to excitation. The areas chosen for different azimuths were also consistent with each other, in agreement with the azimuthal trend they should exhibit according to Eq. (1). This was the case for all except the last azimuth, Ψ = 15°. For that dataset a large degree of domain mixing was apparent in the data, such that a mixture of 105° and 15° domains (90° apart) contributes to the observed intensity. The nonmixed signal for Ψ = 15° was extracted as described in Supplementary Note 4. Contamination between the 60° and 150° azimuths is also possible, but due to their large difference in intensity (see Fig. 3b, c) any appreciable effect would only occur for Ψ = 150°. To account for this, a small fraction (2–4%) of the Ψ = 60° signal is subtracted from the 150° signal before fitting Eq. (1).
Errors in Fig. 4a, b are the standard deviation of the fit values (square root of the diagonal elements of the covariance matrix).
The demagnetizations in the curves in Fig. 4a were fit to an equation of the form
The temporal resolution is estimated at 120 fs. To account for this, fits to Eq. (M3) were conducted with a convolved Gaussian response function of 120 fs width.
Lastly, fits of the transient magnetization direction to the displacive excitation model (Eq. (4)) are done with a constant damping time of τ_{damp} = 150 ps, as this does not affect the results appreciably. Displacive excitations within the DECP model typically yield a phase ζ = 0, due to a steplike shift of the potential minimum, compared to the oscillation response time^{30}. Our response times τ_{φ} are of similar order as the oscillation period (but still shorter than half the oscillation period, as required for displacive excitations), see Fig. 5d. This more gradual shift of the potential leads to a finite oscillation phase ζ between 116° and 97°.
Calculation of absorbed fluence
All fluences reported are total absorbed fluences. In order to determine the optical constants of GdRh_{2}Si_{2}, we conducted reflectivity measurements using 1.55 eV light. From this we estimate the complex index of refraction at this photon energy as n = n_{0} + ik = (3.34 ± 0.10) + (3.19 ± 1.19)i. Using this, recorded incident fluences were corrected for reflection and refraction to produce the total absorbed fluence. Note that a value of 1 mJ cm^{−2} corresponds to an excitation density of 420 J cm^{−3} within the first layer of the material. From this index of refraction, we estimate a penetration depth of 20.6 nm at the Bragg angle θ.
Anisotropy potential
The anisotropy values K presented in Fig. 4f were calculated from the observed oscillations. We first convert them to eigenfrequencies by correcting for the damping as \(\omega _0^2 = \omega^2 + \tau _{\mathrm{damp}}^{−2}\). We then estimate the anisotropy field B_{A} by following the derivation in ref. ^{42} (similarly to ref. ^{31}) as \(\omega _0 = 2\gamma B_{\mathrm{A}}\), with \(\gamma = g\mu _{\mathrm{B}}/h\) and g = 2 for Gd, in which μ_{B} is Bohr’s magneton and h is Planck’s constant. Finally, for a simple estimate of the constant K, we use the relation B_{A} = K/m, in which m is the total Gd 4f moment (μ_{B}g_{J}J), and g_{J} is the Landé factor.
Firstprinciples calculations
The calculations were performed using a firstprinciples Green’s function method within the multiple scattering theory^{43,44} and within the density function theory in a local density approximation^{45}. To correctly describe strongly localized Gd f states, a firstprinciples Hubbard model with U = 3 eV was used^{46}.
The effect of temperature was simulated as a spin disorder using the DLM^{47,48}, implemented using a coherentpotential approximation^{49,50}. In the DLM approach, the absence of spin disorder corresponds to the ground state at T = 0, which is the AF order in the case of GdRh_{2}Si_{2}. An increase of temperature leads to disordering of magnetic moment orientations. A fully disordered moment configuration corresponds to the paramagnetic state high above T_{N}.
The easyaxis direction was calculated as follows. For a given 4f spin disorder level, the spins were aligned (anti)parallel to a given direction in the ab plane. The energy of each spin direction was calculated, and the minimal energy is taken as the easyaxis angle for the given spin disorder.
Reporting summary
Further information on research design is available in the Nature Research Reporting Summary linked to this article.
Data availability
The datasets used in this study are available from the corresponding authors on reasonable request.
References
Jungwirth, T. et al. The multiple directions of antiferromagnetic spintronics. Nat. Phys. 14, 200–203 (2018).
Baltz, V. et al. Antiferromagnetic spintronics. Rev. Mod. Phys. 90, 015005 (2018).
Gomonay, O., Baltz, V., Brataas, A. & Tserkovnyak, Y. Antiferromagnetic spin textures and dynamics. Nat. Phys. 14, 213–216 (2018).
Šmejkal, L., Mokrousov, Y., Yan, B. & MacDonald, A. H. Topological antiferromagnetic spintronics. Nat. Phys. 14, 242–251 (2018).
Schlauderer, S. et al. Temporal and spectral fingerprints of ultrafast allcoherent spin switching. Nature 569, 383–387 (2019).
Bhattacharjee, N. et al. Néel spin–orbit torque driven antiferromagnetic resonance in Mn_{2}Au probed by timedomain THz spectroscopy. Phys. Rev. Lett. 120, 237201 (2018).
Kubacka, T. et al. Largeamplitude spin dynamics driven by a THz pulse in resonance with an electromagnon. Science 343, 1333–1336 (2014).
Kampfrath, T. et al. Coherent terahertz control of antiferromagnetic spin waves. Nat. Photonics 5, 31–34 (2011).
Radu, I. et al. Transient ferromagneticlike state mediating ultrafast reversal of antiferromagnetically coupled spins. Nature 472, 205–209 (2011).
Stupakiewicz, A., Szerenos, K., Afanasiev, D., Kirilyuk, A. & Kimel, A. V. Ultrafast nonthermal photomagnetic recording in a transparent medium. Nature 542, 71–74 (2017).
Železný, J., Wadley, P., Olejník, K., Hoffmann, A. & Ohno, H. Spin transport and spin torque in antiferromagnetic devices. Nat. Phys. 14, 220–228 (2018).
Kliemt, K. et al. GdRh_{2}Si_{2}: an exemplary tetragonal system for antiferromagnetic order with weak inplane anisotropy. Phys. Rev. B 95, 134403 (2017).
Kliemt, K. & Krellner, C. Single crystal growth and characterization of GdRh_{2}Si_{2}. J. Cryst. Growth 419, 37–41 (2015).
SchüßlerLangeheine, C. et al. Resonant magnetic Xray scattering from ultrathin Hometal films down to a few atomic layers. J. Electron Spectros. Relat. Phenom. 114–116, 953–957 (2001).
Fink, J., Schierle, E., Weschke, E. & Geck, J. Resonant elastic soft xray scattering. Rep. Prog. Phys. 76, 056502 (2013).
Hannon, J. P., Trammell, G. T. & M. Blume, D. G. Xray resonance exchange scattering. Phys. Rev. Lett. 61, 2644 (1988).
Hill, J. P. & Mcmorrow, D. F. Xray resonant exchange scattering: polarization dependence and correlation functions. Acta Crystallogr. Sect. A 52, 236–244 (1996).
ColarietiTosti, M. et al. Origin of magnetic anisotropy of Gd metal. Phys. Rev. Lett. 91, 157201 (2003).
Jensen, J. & Mackintosh, A. R. Rare earth magnetism: structures and excitations. 112–113 (Clarendon Press, Oxford, 1991).
Kondorsky, E. A review of the theory of magnetic anisotropy in Ni. IEEE Trans. Magn. 10, 132–136 (1974).
Kirilyuk, A., Kimel, A. V. & Rasing, T. Ultrafast optical manipulation of magnetic order. Rev. Mod. Phys. 82, 2731–2784 (2010).
ThielemannKühn, N. et al. Ultrafast and energyefficient quenching of spin order: antiferromagnetism beats ferromagnetism. Phys. Rev. Lett. 119, 197202 (2017).
Rettig, L. et al. Itinerant and localized magnetization dynamics in antiferromagnetic Ho. Phys. Rev. Lett. 116, 257202 (2016).
Wietstruk, M. et al. Hotelectrondriven enhancement of spin–lattice coupling in Gd and Tb 4f ferromagnets observed by femtosecond xray magnetic circular dichroism. Phys. Rev. Lett. 106, 127401 (2011).
Eschenlohr, A. et al. Role of spin–lattice coupling in the ultrafast demagnetization of Gd_{1−x}Tb_{x} alloys. Phys. Rev. B 89, 214423 (2014).
Koopmans, B. et al. Explaining the paradoxical diversity of ultrafast laserinduced demagnetization. Nat. Mater. 9, 259–265 (2010).
Roth, T. et al. Temperature dependence of laserinduced demagnetization in Ni: a key for identifying the underlying mechanism. Phys. Rev. X 2, 021006 (2012).
Frietsch, B. et al. Disparate ultrafast dynamics of itinerant and localized magnetic moments in gadolinium metal. Nat. Commun. 6, 8262 (2015).
Atxitia, U. & ChubykaloFesenko, O. Ultrafast magnetization dynamics rates within the Landau–Lifshitz–Bloch model. Phys. Rev. B 84, 144414 (2011).
Zeiger, H. et al. Theory for displacive excitation. Phys. Rev. B 45, 768–778 (1992).
Sichelschmidt, J., Kliemt, K., HofmannKliemt, M. & Krellner, C. Weak magnetic anisotropy in GdRh_{2}Si_{2} studied by magnetic resonance. Phys. Rev. B 97, 214424 (2018).
Brorson, S. D. et al. Femtosecond roomtemperature measurement of the electron–phonon coupling constant γ in metallic superconductors. Phys. Rev. Lett. 64, 2172–2175 (1990).
Low, G. G., Okazaki, A., Stevenson, R. W. H. & Turberfield, K. C. A measurement of spinwave dispersion in MnF_{2} at 4.2°K. J. Appl. Phys. 35, 998 (1964).
Olejník, K. et al. Terahertz electrical writing speed in an antiferromagnetic memory. Sci. Adv. 4, 3 (2018).
Corner, W. D. & Tanner, B. K. The easy direction of magnetization in gadolinium. J. Phys. C 9, 627–633 (1975).
Flechsig, U. et al. Performance measurements at the SLS SIM beamline. AIP Conf. Proc. 1234, 319–322 (2010).
Staub, U. et al. Polarization analysis in soft Xray diffraction to study magnetic and orbital ordering. J. Synchrotron Radiat. 15, 469–76 (2008).
Brookes, N. B. et al. The beamline ID32 at the ESRF for soft Xray high energy resolution resonant inelastic Xray scattering and polarisation dependent Xray absorption spectroscopy. Nucl. Instrum. Methods Phys. Res. Sect. A 903, 175–192 (2018).
Aharoni, A. lntroduction to the Theory of Ferromagnetism (Oxford Univ. Press, 1996).
Pontius, N., Holldack, K., SchüßlerLangeheine, C., Kachel, T. & Mitzner, R. The FemtoSpeX facility at BESSY II. J. largescale Res. Facil. 2, A46 (2016).
Schick, D. et al. Analysis of the halo background in femtosecond slicing experiments. J. Synchrotron Radiat. 23, 700–711 (2016).
Gurevich, A. G. & Melkov, G. A. Magnetization Oscillations and Waves (CRC Press, Boca Raton, 1996).
Gyorffy, B. L. & Stott, M. J. in Proc. International Conference on Band Structure and Spectroscopy of Metals and Alloys (eds Fabian, D. J. & Watson, L. M.) 385–402 (Academic Press, London and New York, 1973).
Geilhufe, M. et al. Numerical solution of the relativistic singlesite scattering problem for the Coulomb and the Mathieu potential. J. Phys. Condens. Matter 27, 435202 (2015).
Perdew, J. P. et al. Atoms, molecules, solids, and surfaces: applications of the generalized gradient approximation for exchange and correlation. Phys. Rev. B 46, 6671–6687 (1992).
Anisimov, V. I., Zaanen, J. & Andersen, O. K. Band theory and Mott insulators: Hubbard U instead of Stoner I. Phys. Rev. B 44, 943–954 (1991).
Gyorffy, B. L., Pindor, A. J., Staunton, J., Stocks, G. M. & Winter, H. A firstprinciples theory of ferromagnetic phase transitions in metals. J. Phys. F 15, 1337 (1985).
Staunton, J., Gyorffy, B. L., Pindor, A. J., Stocks, G. M. & Winter, H. Electronic structure of metallic ferromagnets above the Curie temperature. J. Phys. F 15, 1387 (1985).
Soven, P. Coherentpotential model of substitutional disordered alloys. Phys. Rev. 156, 809–813 (1967).
Gyorffy, B. L. Coherentpotential approximation for a nonoverlappingmuffintinpotential model of random substitutional alloys. Phys. Rev. B 5, 2382–2384 (1972).
Acknowledgements
We gratefully acknowledge the experimental support of the staff at beamlines UE56/1 (HZB), X11MA (SLS), and ID32 (ESRF). This work received funding from the DFG within the Emmy Noether programme under Grant No. RE 3977/1, within the Transregio TRR 227 Ultrafast Spin Dynamics (Projects A09 and A03) and within Grant No. KR3831/51. We acknowledge financial support from the Spanish Ministry of Economy (MAT201788374P). Open access funding provided by Projekt DEAL.
Author information
Authors and Affiliations
Contributions
L.R. and D.V.V. planned the experiment. K.Kl. and C.K. grew the crystals. Equilibrium RXD experiments were performed by Y.W.W., K.K., U.S. and L.R., and analysed by Y.W.W. and K.K. Firstprinciples calculations were done by A.E. Timeresolved RXD experiments were performed by Y.W.W., L.R., C.S.L. and N.P., and analysed by Y.W.W. and L.R. Interpretation was done by Y.W.W., L.R., A.E. and E.V.C. The manuscript was written by Y.W.W. and L.R. All authors contributed to discussion and revision of the manuscript to its final version.
Corresponding authors
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Windsor, Y.W., Ernst, A., Kummer, K. et al. Deterministic control of an antiferromagnetic spin arrangement using ultrafast optical excitation. Commun Phys 3, 139 (2020). https://doi.org/10.1038/s42005020004070
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s42005020004070
This article is cited by

Exchange scaling of ultrafast angular momentum transfer in 4f antiferromagnets
Nature Materials (2022)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.